1 / 45

450 likes | 616 Vues

Department of Mechanics and Physics of Fluids. T. A. Kowalewski S. Błoński S. Barral. Experiments and Modelling of Electrospinning Process. NANOFIBRES. Nanofibres background. Nanofibres properties Increase of the surface to volume ratio -> solar and light sails and mirrors in space

Télécharger la présentation
## T. A. Kowalewski S. Błoński S. Barral

**An Image/Link below is provided (as is) to download presentation**
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.
Content is provided to you AS IS for your information and personal use only.
Download presentation by click this link.
While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
During download, if you can't get a presentation, the file might be deleted by the publisher.

E N D

**Department of Mechanics and Physics of Fluids**T. A. Kowalewski S. Błoński S. Barral Experiments and Modelling of Electrospinning Process NANOFIBRES**Nanofibres background**• Nanofibres properties • Increase of the surface to volume ratio -> solar and light sails and mirrors in space • Reduction of characteristic dimension -> nano-biotechnology, tissue engineering, chemical catalysts, electronic devices • Bio-active fibres: catalysis of tissue cells growth • Mechanical properties improvement -> new materials and composite materials by alignment in arrays and ropes • Nanofibres production: • Air-blast atomisation • Pulling from melts • Electrospinning of polymer solutions NANOFIBRES, CDMM2005, Warsaw, Poland**Classical liquid jet** 0.1mm Orifice – 0.1mm Primary jet diameter ~ 0.2mm Micro-jet diameter ~ 0.005mm • Gravitational, mechanical or • electrostatic pulling limited to • l/d ~ 1000 by capillary instability • To reach nano-range: • jet thinning ~10-3 • draw ratio ~106 ! NANOFIBRES, CDMM2005, Warsaw, Poland**Electro-spinning**v=0.1m/s moving charges e bending force on charge e E ~ 105V/m viscoelastic and surface tension resistance Moving charges (ions) interacting with electrostatic field amplify bending instability, surface tension and viscoelasticity counteract these forces NANOFIBRES, CDMM2005, Warsaw, Poland**Electro-spinning**bending instability of electro-spun jet charges moving along spiralling path E ~ 105V/m Bending instability enormously increases path of the jet, allowing to solve problem: how to decrease jet diameter 1000 times or more without increasing distance to tenths of kilometres NANOFIBRES, CDMM2005, Warsaw, Poland**Electro-spinning**Simple model for elongating viscoelastic thread Stress balance: - viscosity, G – elastic modulus stress, stress tensor, dl/dt – thread elongation Momentum balance: Vo – voltage, e – charge, a – thread radius, h- distance pipette-collector Kinematic condition for thread velocity v Non-dimensional length of the thread as a function of electrostatic potential NANOFIBRES, CDMM2005, Warsaw, Poland**Nanofibres – basic setup**liquid jet ~ 105 Volt/m NANOFIBRES, CDMM2005, Warsaw, Poland**Nanofibres – howto?**• Viscoelastic fluid: • Dilute solution (4 – 6)% of polyethylene oxide (molar weight 4.105 g/mol), in 40% ethanol –water solvent • Electrostatic field • high voltage power supply (5-30kV) • plastic syringe • metal grid to collect fibres • Visualization • high speed camera (4000 – 40000 fps) • high resolution „PIV” camera (1280x1024pixels) • CW Argon laser, double pulse Nd:Yag laser, projection lens NANOFIBRES, CDMM2005, Warsaw, Poland**Nanofibres – basic setup**NANOFIBRES, CDMM2005, Warsaw, Poland**Nanofibres collection**NANOFIBRES, CDMM2005, Warsaw, Poland**Nanofibres collection**NANOFIBRES, CDMM2005, Warsaw, Poland**Electrospinning observed at 30fps**Average velocity of the fibres: 2 m/s 5 cm NANOFIBRES, CDMM2005, Warsaw, Poland**Electrospinning observed at 4500fps**NANOFIBRES, CDMM2005, Warsaw, Poland**Electrospinning observed at 4500fps**Average velocity of the fibre: 2 m/s 5 cm NANOFIBRES, CDMM2005, Warsaw, Poland**Electron microscopy**PEO nanofibres NANOFIBRES, CDMM2005, Warsaw, Poland**Parametric study**• Model validation varying following parameters: • L – length of the rectilinear part • – angle of the envelope cone (image analysis) • U – velocity of the fibre by PIV method • a – fibre diameter (image analysis) • structure of collected woven (failure modes) • elongation strength of single fibre measured by air jet • Effect of • Electrostatic potential V • Distance pipette-collector H • Solution concentration c • Distance from the pipette x L H NANOFIBRES, CDMM2005, Warsaw, Poland**Parametric study**PIV cross – correlation t = 500 s image 2 t + t image 1 • concentration of PEO: 3% • Voltage: 8 kV • H = 215 mm • polymer solution with the addition of fluorescent particles • (0.3m polymer microspheres) • light source: Nd:Yag laser Average velocity of the fibres: 2 m/s NANOFIBRES, CDMM2005, Warsaw, Poland**Tested polymers**NANOFIBRES, CDMM2005, Warsaw, Poland**Parametric study**L H • Polymer: PEO • Concentration: c=3% • Solvent: 40% water- ethanol solution • H=215mm • V=8kV • L (t) – instability of length of the rectilinear part NANOFIBRES, CDMM2005, Warsaw, Poland**Parametric study**L H • Polymer: PEO • Concentration: c=4% • Solvent: 40% water- ethanol solution • H=215mm • L (V) – length of the rectilinear part • (V) – angle of the envelope cone NANOFIBRES, CDMM2005, Warsaw, Poland**Parametric study**L H • Polymer: PEO • Concentration: c=4% • Solvent: 40% water- ethanol solution • H=215mm • U(V) – velocity of the fibre at the rectilinear part NANOFIBRES, CDMM2005, Warsaw, Poland**Electrospinning observed at 25fps**• Polymer: DBC • Concentration: c=9% • Solvent: ethanol • H=215mm • V=6kV 12 cm NANOFIBRES, CDMM2005, Warsaw, Poland**Different structure of spinning fibres for DBC polymer**U=6kV U=12kV DBC: c=9%H=215mm NANOFIBRES, CDMM2005, Warsaw, Poland**Parametric study**L H • Polymer: DBC • Concentration: c=9% • Solvent:ethanol • H=215mm • L (V) – length of the rectilinear part • (V) – angle of the envelope cone NANOFIBRES, CDMM2005, Warsaw, Poland**Electrospinning observed at 25fps**• Polymer: PAN • Concentration: c=15% • Solvent: DMF • H=215mm • V=13kV 12 cm NANOFIBRES, CDMM2005, Warsaw, Poland**Different structure of spinning fibres for PAN polymer**U=13kV U=19kV PAN: c=15%H=215mm NANOFIBRES, CDMM2005, Warsaw, Poland**Parametric study**L H • Polymer: PAN • Concentration: c=15% • Solvent: DMF • H=215mm • L (V) – length of the rectilinear part • (V) – angle of the envelope cone NANOFIBRES, CDMM2005, Warsaw, Poland**Electrospinning of Glycerol**• Glycerol • Concentration: c=88% • Solvent: water • H=215mm • V=20kV 12 cm NANOFIBRES, CDMM2005, Warsaw, Poland**Comparison of PEO & DBC &PAN polymers**PEO DBC PAN • L (V) – length of the rectilinear part • (V) – angle of the envelope cone NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model Main assumptions**• The electric field created by the generator is considered static and isapproximated using a sphere-plate capacitor configuration • The fibre is a perfect insulator with a constant electric charge density distributed over its surface • The melt is viscoelastic and has constant elastic modulus, viscosity and surface tension NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model**2. Governing equations a – surface tension l – stretching parameter (relative elongation) – viscosity r – density – longitudinal stress a – radius of the fiber C – short-range E-field cutoff factor E – electric field G – elastic modulus q – charge per unit length r – coordinate vector s – Lagrangian curvilinear coordinate u – unit vector along the fiber V – velocity vector • Mass conservation: • Stress balance • Momentum balance NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model**3. Discretized equations • Mass conservation: • Stress balance • Momentum balance NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model**4. Boundary conditions The last particle introduced at the tips keeps a constant velocity until the distance to the tip exceeds the initial bead length l0: A small perturbation is added to the position of each new particle introduced near the tip: Particles that reach the collector are considered neutralized and are removed from the fibre. l0 – initial bead length [input] Q – volume flow rate [input] e – distance to the main axis [input] j – random phase NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model**5. Parametric simulations Reference case: a = 0.07 N/m F = 5000 V = 10 Pa.s G = 105 Pa r = 1000 kg/m3 a0 = 150 μm H = 20 cm l0 = 1 μm q = 200 C/m3 Q = 3.6 cm3/h a F m G Case 3 1 /3 2 3 x2 4 x5 5 x2 /2 6 NANOFIBRES, CDMM2005, Warsaw, Poland**a = 0.07 N/m**F = 5000 V = 10 Pa.s G = 105 Pa r = 1000 kg/m3 a0 = 150 μm H = 20 cm l0 = 1 μm q = 200 C/m3 Q = 3.6 cm3/h Numerical model Reference case: NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model**Reference case NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model**Triple surface tension NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model**1/3 surface tension NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model**½ Voltage NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model**5 times higher viscosity NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model**Double elastic modulus NANOFIBRES, CDMM2005, Warsaw, Poland**Numerical model**Half elastic modulus NANOFIBRES, CDMM2005, Warsaw, Poland**a = 0.07 N/m**F = 5000 V = 10 Pa.s G = 105 Pa r = 1000 kg/m3 a0 = 150 μm H = 20 cm l0 = 1 μm q = 200 C/m3 Q = 3.6 cm3/h Numerical model Reference case: a = 0.21N/m a = 0.023N/m F = 2500V = 2 Pa.s G = 2.105 Pa G = 5.104 Pa NANOFIBRES, CDMM2005, Warsaw, Poland**Conclusions**• Electrostatic elongation of polymer threads allows to produce relatively easily fibres in nano range diameters • Collection of nano-woven of bio-active polymers, e.g.. chitin may have practical application for tissue growth • Simulations recover some key physical phenomena but fail at modelling the straight jet portion • The modeling of electrospun fibers is still embryonic. Improvements are required in many areas: - better physical description (evaporation, varying viscosity, ...) - checking of the mathematical correctness of the model (is the discrete charge model fully consistent?) - development of a fast algorithm for Coulomb interactions - ... NANOFIBRES, CDMM2005, Warsaw, Poland**Acknowledgements**We would like to acknowledge the valuable contribution of dr Anna Błasińska from TU of Łódź and Anna Blim from IPPT PAN in the work presented. NANOFIBRES, CDMM2005, Warsaw, Poland

More Related